Four new silver phosphonates constructed from semi-rigid phosphonate ligands: syntheses, structures and properties
Hou, Xiaomin; Tang, Sifu; RSC Adv.  (2016) –; doi:10.1039/C6RA21382K

data_7226806
_publ_section_title
;
 Four new silver phosphonates constructed from semi-rigid phosphonate
 ligands: syntheses, structures and properties
;
_journal_name_full               'RSC Adv.'
_journal_paper_doi               10.1039/C6RA21382K
_journal_year                    2016
_chemical_formula_sum            'C9 H12 Ag3 O9 P3'
_chemical_formula_weight         680.71
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2013
_audit_update_record
;
2016-08-12 deposited with the CCDC.
2016-10-17 downloaded from the CCDC.
;
_cell_angle_alpha                86.327(4)
_cell_angle_beta                 89.491(4)
_cell_angle_gamma                63.771(3)
_cell_formula_units_Z            2
_cell_length_a                   8.3751(9)
_cell_length_b                   9.2734(9)
_cell_length_c                   10.7848(13)
_cell_measurement_reflns_used    8206
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.481
_cell_measurement_theta_min      3.199
_cell_volume                     749.64(14)
_computing_cell_refinement       'Bruker XSCANS'
_computing_data_collection       'Bruker XSCANS'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.986
_diffrn_measured_fraction_theta_max 0.950
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0588
_diffrn_reflns_av_unetI/netI     0.0703
_diffrn_reflns_Laue_measured_fraction_full 0.986
_diffrn_reflns_Laue_measured_fraction_max 0.950
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            8206
_diffrn_reflns_point_group_measured_fraction_full 0.986
_diffrn_reflns_point_group_measured_fraction_max 0.950
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.481
_diffrn_reflns_theta_min         3.199
_exptl_absorpt_coefficient_mu    4.246
_exptl_absorpt_correction_T_max  0.809
_exptl_absorpt_correction_T_min  0.360
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.016
_exptl_crystal_description       plate
_exptl_crystal_F_000             648
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.05
_refine_diff_density_max         0.887
_refine_diff_density_min         -0.906
_refine_diff_density_rms         0.172
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.006
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     217
_refine_ls_number_reflns         2951
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.006
_refine_ls_R_factor_all          0.0799
_refine_ls_R_factor_gt           0.0386
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
;
 w=1/[\s^2^(Fo^2^)+(0.0229P)^2^+0.2057P]
 where P=(Fo^2^+2Fc^2^)/3
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0580
_refine_ls_wR_factor_ref         0.0670
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2013
_reflns_number_total             2951
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c6ra21382k2.cif
_cod_data_source_block           1
_cod_database_code               7226806
_shelxl_version_number           2013-2
_shelx_res_checksum              58159